COLORING CONCRETE ENERGIZED BY PROCESSING INSTRUCTIONS COLORING CONCRETE PROCESSING INSTRUCTIONS Concrete is a modern material that offers urban plan­ ners, architects and builders a variety of creative op­ tions for the design of urban environments and infra­ structure. Using inorganic pigments to color ­materials such as concrete pavers and roofing tiles also pro­ duces solutions with esthetic appeal that integrate harmoniously into the surroundings. The method of production differs only slightly from that of corre­ sponding uncolored products. In order to obtain the best possible result, however, there are a number of important details that need to be considered when ­using pigments. 2 This brochure summarizes the results of laboratory trials with colored concrete carried out by LANXESS. It also takes ­account of building industry experience. The aim is to help users of inorganic pigments in concrete to manufacture ­ high-quality end-products. LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete CONTENTS Coloring concrete: Processing instructions2 Components required for manufacturing colored concrete products The pigment 5 Influence of the formulation on the color of concrete The cement The aggregates 9 Manufacture of colored concrete products Metering and dispersion of pigments in concrete 14 Weathering behavior of pigmented concrete 16 Technical properties of colored concrete 18 Standards Concrete consistency Quality and added value for customers 19 LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 3 4 LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete COMPONENTS REQUIRED FOR MANUFACTURE The pigment The choice of pigment is of major importance for the quality of the end product. Years of observing colored con­ crete products exposed to different location- and climate-specific conditions have shown that inorganic oxide pigments exhibit particularly high durability due to their color stability and resistance properties. LANXESS markets these oxide pigments worldwide under the names Bayferrox® and Colortherm®. Bayferrox® pigments – sustainability and the environment The introduction of quality hallmarks for sustainable products in many sectors clearly demonstrates the broad consensus in our society as regards the need to handle the resources available to us responsibly. Sustainability is a key issue and customers not only appreciate sustainable behavior, but have come to expect it. Sustainable and responsible environmental and social behavior is an integral part of LANXESS’s corporate strategy. Products and production processes are designed to conserve resources and preserve the environment – and to be safe and sustainable. They are also subject to continuous improvement. Our Bayferrox® iron oxide and Colortherm® chromium oxide green pigments are neither toxic nor do they irritate the skin or mucous membranes. From an environmental and health protection perspective, they are ideal for coloring building materials, although the generation of dust should be avoided for occupational health reasons. Although the insolubility of Bayferrox® and Colortherm® pigments means they are not harmful to aquatic organisms, they do result in significant discoloration of water. Any pigments that are spilled should therefore always be cleaned up, either by wet or dry method. Prerequisites of pigments used for the coloring of concrete Oxide pigments are perfect for coloring building materials. Due to their chemical composition and structure, they are insoluble in water and dilute acids, resistant to lime and alkalis, and completely weather- and light-stable. Which shades can be produced? The oxide pigments suitable for coloring building materials cover all the most popular colors. These shades are similar to colors occurring in nature, which means they blend into their surroundings: Red: Yellow: Brown: Black: Yellowish to bluish red Greenish to reddish yellow Light to dark brown/red brown Dark gray to anthracite Shades of white, green and blue can also be produced, while pure colors such as yellow can be made using white cement. However, the options for producing brilliant shades, like those achieved in plastics and surface coatings, are very ­limited due to the composition and surface texture of concrete. Fig. 1: Overview of the most important­ oxide pigments Color Name LANXESS brand name Black Iron oxide black Bayferrox®-Black Red Iron oxide red Bayferrox®-Red Yellow Iron oxide yellow Bayferrox®-Yellow Brown Iron oxide brown Bayferrox®-Brown Green Chromium oxide Colortherm® Green Blue Cobalt blue – White Titanium dioxide – LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 5 The tinting strength of pigments The tinting strength of pigments is an important quality characteristic that is essential in evaluating their cost-effectiveness. A pigment’s tinting strength is its ability to transfer its inherent color to the medium being colored. The graphic below shows an example: two seemingly equally red powders – brick dust on the left and a Bayferrox® Red pigment on the right. The difference in the two samples’ tinting strength only becomes apparent when they are used to color concrete or tested in the laboratory. The above-mentioned laboratory test is performed in accordance with EN 12 878 and is the basis for the tinting strength tolerances given in the product specification for B ­ ayferrox® pigments.­ Comparing pigments with low and high tinting strengths Taking the practical example of a concrete factory: An iron ­oxide red pigment “A” has been offered. A 6 % concentration of this pigment is required to obtain a given shade. As the samples shown here demonstrate, however, it is also possible to obtain the desired shade by adding 3 % of red pigment “B”. Fig. 3: Comparison of pigments’ tinting strength 3% 6% Pigment A (low tinting strength) Fig. 2: Comparison of pigments’ tinting strength Pigment B (high tinting strength) 3% Brick Pigment Conclusion: Price alone says little about cost-effectiveness. Even if pigment “A” is cheaper, the additional quantity needed to obtain the desired shade may mean it is the much less cost-effective option. 6 LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete Color consistency Another extremely important quality criterion for pigments alongside tinting strength is color consistency – i. e. ­whether­ there are differences in color between different deliveries (Fig. 4). Thanks to state-of-the-art production facilities and painstaking quality control, LANXESS has been offering its customers absolute color consistency in its end products for decades. Fig. 4: Color consistency Batch 1 Batch 2 Batch 3 Supplier 1 Supply forms Pigment processability requirements have changed over the years. Initially, most of the pigments used in the construction industry were powder pigments, then waterborne pigment slurries subsequently became established in the market. Besides the complete absence of dust, these slurries offer processors the benefit of easy handling and metering. However, they have a relatively high water content, which means that they cost more to transport than powder pigments. In addition, the pigment may settle if suspensions are not ­periodically stirred if they are stored for a prolonged period of time. For the above-mentioned reasons, it only makes sense to purchase ready-made pigment suspensions if located ­within a certain distance from the supply plant. Free-flowing dry pigment preparations are the most recent supply form to be developed. They facilitate the easy emptying of silos, sacks and bulk bags, and only a minimal amount of dust is generated during transfer and metering. Further details about supply forms and packaging are available on request. Supplier 2 Fig. 5: Light micrographs (100 x magnification) of Bayferrox® pigments Powder Compact pigment Granules LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 7 INFLUENCE OF THE FORMULATION ON THE COLOR OF CONCRETE The cement Gray cement is still used for most construction projects, which has implications for the possible coloring o ­ ptions. Unlike white cement, gray cement takes the brilliance out of all colors. As a result, bright, radiant colors cannot be obtained in pigmented concrete manufactured using ordinary Portland cement. However the gain in color purity yielded by using white ­cement depends on the pigment used. In the case of black pigments, there is virtually no difference between products made using white or gray cement. The difference is slight when working with dark brown and red pigments, but very pronounced with yellow and green ones. The brighter and cleaner the desired shade, the greater the dependency on white cement. Even a layperson can easily understand this difference in coloring white and gray cement. However, specialists also need to know that gray cement can vary in color from light to dark gray. When changing cement type or supplier, these differences in the inherent color of cement may often influence the shade of the concrete as well. Fig. 6: Influence of the cement color on the shade of the concrete 4% Bayferrox® 610 4% Bayferrox® 110 4% Bayferrox® 920 4% Bayferrox® 318 4% Colortherm® Green GN White cement Gray cement 8 LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete The aggregates When manufacturing colored concrete, the aggregate particles are covered by the pigmented cement paste. The particles of a highly pigmented aggregate may not be completely covered, with the result that the inherent color of the aggregate affects the color of the end product. This effect is ­already apparent when producing colored concrete. However, the influence of the aggregate’s inherent color becomes even more evident when weathering and surface erosion expose the aggregate particles. The human eye then sees a composite shade made up of the color of the hardened cement matrix and that of the exposed aggregate. Like cement, the inherent color of the sand also has a more noticeable effect on light-colored concrete (e. g. yellow, green) than on dark concrete (e. g. brown, black). Fig. 7: Influence of the aggregate color on the shade of the concrete 4% Bayferrox® 610 4% Bayferrox® 110 4% Bayferrox® 920 4% Bayferrox® 318 4% Colortherm® Green GN Light aggregates Dark aggregates Daum Kakao Space. 1, Jeju Island, Korea; pigmented with ­Bayferrox® 318, 4130 and 920 LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 9 Influence of the pigment addition rate on the shade of the concrete Knowing the optimal pigment addition rate is a key ­economic­ and technical factor. It helps achieve transparency regarding the costs of coloring concrete and is also essential to producing the desired shade and intensity. the system parameters of the concrete. However, ­generally­ speaking, pigment additions above 5 % (relative to the amount of binder) are not necessary for Bayferrox® pigments due to their high tinting strength. Adding increasing amounts of pigment to a concrete mixture initially results in a linear increase in color intensity in line with the pigment concentration. As more pigment is added, however, a point comes at which the addition of ­further pigment does not significantly deepen the shade and is therefore ­uneconomical. The saturation range is determined in part by In the case of pigments with a lower tinting strength, on the other hand, the saturation range is reached only after adding much larger amounts of pigment. The amount of pigment ­required to produce a given shade can thus sometimes be so large that the increase in the quantity of fines has a negative effect on the concrete’s technical properties. Fig. 8: Influence of pigmentation level on final shade Bayferrox® 920 Bayferrox® 110 Bayferrox® 318 Saturation point 0% 4% Color 2% 6% 8% 0 1 2 3 4 5 6 7 Pigment concentration [%], calculated on the pigment Bayferrox® 318 Water-cement ratio and the color of concrete When drinking a glass of beer, you may have wondered why the foam is white although the beer itself is amber in color? The foam is made up of countless tiny air bubbles, which scatter the light in the same way as white pigments. This ­digression is important as it explains the relationship between the color of the concrete and its water-cement ratio. 10 Bayferrox® 110 8 Bayferrox® 920 The excess mixing water evaporates from the concrete, leaving behind cavities in the form of fine pores. These act like the bubbles in the beer foam. They scatter the incident light and thus lighten the color of the concrete. The higher the ­ water-cement ratio, the lighter the concrete appears. As the following photo shows, unpigmented gray concrete is ­affected­just as much by this phenomenon as pigmented concrete. LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete Fig. 9: Influence of water-cement ratio on color of concrete W/C ratio 0.30 W/C ratio W/C ratio 0.35 0.40 unpigmented 4 % Bayferrox® 610 N For this reason, color fluctuations that occur on a production line due to the water-cement ratio tend to be the exception rather than the rule. On the other hand, the differences in shade can be substantial if the excessive moisture in the concrete results in the formation of a thick layer of sludge on the surface of the concrete. This sludge – called “orange peel” in paving block manufacture – contains the very fine components of the concrete such as cement, fines and an above-average accumulation of pigment. As a result, the concrete has a different appearance than if there was a thin layer of sludge on the surface. The color of concrete in relation to cement content When coloring concrete, it is not the aggregate that is pigmented but the cement paste, which then forms a layer around the individual aggregate particles. What does this mean in practice? When comparing the color of concrete with very different ­water contents (e. g. concrete pavers and in-situ concrete), the color of the samples differs although the pigment addition rate is the same. Fig. 10: Color impression in different applications Mortar Exposed concrete Wetcast Paver In considering whether the cement content of the colored concrete influences its color, we assume for the sake of simplicity that it is a two-substance mixture comprising colored cement paste and aggregate. The more the colored cement paste is “diluted” with aggregate, the less intense the color of the concrete is. This theory is confirmed in practice. C ­ oncrete with a high cement content will have a much stronger color than concrete with the same pigment concentration – which is normally calculated as a percentage by weight of the ­cement – but a lower cement content. Fig. 11: The color of concrete in relation to cement content 4% Bayferrox® 920 4% Bayferrox® 110 4% Bayferrox® 318 330 kg/m3 Pigment addition rate in all samples: 3 % Bayferrox® 330 450 kg/m3 A different picture emerges for comparisons within a particular product line. Consistency usually has to be kept within narrow limits to ensure trouble-free processing of the concrete in a concrete manufacturing unit, which means that the manufacturer normally needs to meter the mixing water very carefully LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 11 THE MANUFACTURE OF COLORED CONCRETE PRODUCTS The metering and dispersion of pigments in concrete Quality is increasingly important nowadays. For this reason, the metering and dispersion of pigments are key criteria in the building industry, because high-quality colored concrete products cannot be produced without precise metering and the thorough and homogeneous dispersion of pigments. Once pigment consumption at a concrete factory has reached a certain level, the next logical question is whether the addition process can be automated. As is often the case with technical solutions, there are both advantages and disadvantages. There is no one single answer to the question of ­whether wet or dry metering is better. All that can be done is to provide suggestions which, together with precise knowledge of local conditions and consideration of various commercial ­aspects, can help in the decision-making process. Besides the o ­ bvious ­advantages of automatic pigment metering, concrete manufacturers can add further colors to their product line. B ­ ayferrox® pigments are available in the primary colors red, black and yellow. Various shades of each color are also available. Combining two or three B ­ ayferrox® pigments enables the creation of a virtually unlimited number of additional shades. Present-­day concrete mixing technology allows several individual pigments to be added directly and simultaneously to the mixer. There is no need to premix the pigments. Dispersion of pigments in concrete As already explained, pigments are very fine products. Like other fine powders, they tend to form loose clumps during transportation and storage. Although these clumps of pigment are relatively soft and easy to break down, they may survive the mixing process intact if mixing conditions are unfavorable. This has a particularly unattractive effect if the clumps of pigment are visible on the surface of the concrete, as can be clearly seen in Fig. 12. 12 Fig. 12: Paver with lumps of pigment on the surface As a result, the mixing process is a vital aspect of manufacturing concrete. In addition to the usual requirements, i.e. optimal dispersion of all other components to maximize strength, good dispersion is the only way of ensuring evenly colored concrete. Given that mixing times can nowadays be extremely short, it is of the utmost importance to add components during the mixing process in an order that ensures clumps of pigment are broken down and pigment particles are dispersed effectively in the mixture. Lab tests and practical experience have shown that good results are always achieved if the pigment is premixed with the aggregate for around 15 – 30 seconds before the cement is added and this is followed by dry mixing for a further 15 – 30 seconds. The mixing process is otherwise the same as for unpigmented concrete. Adding all of the components simultaneously or mixing in the cement immediately after the sand should be avoided at all costs. LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete Fig. 13: Recommended mixing sequence when manufacturing colored concrete aggregates + pigment 10 20 aggregates + pigment + cement 30 40 50 aggregates + pigment + cement + water 60 70 80 90 100 110 120 130 140 150 160 170 Total mixing time [s] Of course, the mixing time also plays a role in determining whether or not homogeneous dispersion of the pigment is achieved. Each type of mixer has a minimum mixing time requirement. In the case of forced circulation mixers, this is around 1.5 – 2 minutes. Any shorter and it is impossible to achieve a homogeneous mixture, even if the mixing times of the individual c­ omponents or the order in which these are added is changed. The influence of curing conditions on the shade of concrete The cured cement matrix, which is formed from the ­reaction between the mixing water and the cement, forms crystals of varying size, depending on the temperature at which the concrete is cured. The size of these crystals is, in turn, responsible for scattering the light that falls onto the concrete. The following principle applies: Higher curing temperatures result in finer crystal needles. The stronger light scattering resulting from the fine crystal needles makes the color of the concrete lighter than that of the same concrete cured at a lower temperature. However, this ­ phenomenon generally only becomes apparent when the difference in temperature ­reaches a certain magnitude, for example when steam-­cured concrete is compared with concrete cured at normal room temperature and humidity. Fig. 14 illustrates these behavior patterns. It compares the coloring of concrete cured at 5 °C and 35 °C. Fig. 14: The influence of curing conditions on the shade of colored concrete 5 °C 35 °C unpigmented 4% Bayferrox® 318 4% Bayferrox® 663 4% Bayferrox® 130 4% Bayferrox® 920 LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 13 One final important point regarding how pigments should be measured and metered: color pigments are very fine­ powders (around ten times finer than cement) and very sensitive in terms of compressibility. This means that the bulk density of fine ­powders can vary due to all kinds of external influences (such as storage and transportation conditions). In the case of volumetric measurement of powder pigments, it is therefore entirely possible for the volumes measured to be the same but for the quantity of pigment to differ in terms of weight. The differences in color this causes can easily be avoided by using weight-based measurement. 14 unpressed powder pigment compresed powder pigment 115 cm 98 cm Actual height dependent on ­pigment type and bag fill-weight Actual height dependent on ­pigment type and bag fill-weight Fig. 15: Comparison between volumetric and gravimetric measurement 130 IIIIIIIII PO721410P002 25 kg 130 IIIIIIIII PO721410P002 25 kg 130 IIIIIIIII PO721410P002 25 kg 130 IIIIIIIII PO721410P002 25 kg 130 IIIIIIIII PO721410P002 25 kg 130 IIIIIIIII PO721410P002 25 kg 130 IIIIIIIII PO721410P002 25 kg 130 IIIIIIIII PO721410P002 25 kg LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete Volumetric metering Gravimetric metering Amount of pigment: 1500 cm3 (= 1200 g) Amount of pigment: 1200 g Amount of pigment: 1500 cm3 (= 1350 g) Amount of pigment: 1200 g WEATHERING BEHAVIOR OF COLORED CONCRETE The Roman aqueduct that supplied the German city of Cologne with water from the Eifel hills two thousand years ago was built using trass cement. Had this ancient “concrete” been pigmented with natural iron oxides – which were already known at the time – the structure, parts of which can still be visited, would still be colored today. The difference from the original shade would be quite small. There are various reasons for these color changes, which occur in both colored and uncolored concrete. They may be temporary (e. g. efflorescence) or permanent (e. g. exposure of aggregate). Efflorescence on concrete Efflorescence is the curse of all concrete manufacturers, ­especially if color is involved and particularly high standards are specified for the appearance of the concrete. It is important to note that neither Bayferrox® nor ­Colortherm® pigments have any influence on the occurrence of efflorescence. By their very nature, however, white lime deposits are more noticeable on colored concrete than on natural gray or white concrete. Efflorescence results from the formation of free lime when the cement sets. Dissolved in the mixing ­water (primary efflorescence) or in external water such as rain or dew (secondary efflorescence), the lime migrates to the ­surface of the concrete, where it reacts with carbon dioxide in the air to form insoluble calcium carbonate. The porosity of the concrete also plays an important role. The denser it is, the less likely efflorescence will occur. Fig. 16: Efflorescence Unweathered After a few weeks After 1 – 2 years After a few years Concrete roofing In a slow reaction, the calcium carbonate on the surface of the concrete reacts with carbon dioxide dissolved in water to form calcium bicarbonate, which is in turn soluble in ­water. The efflorescence is thus weathered away. Acidic components in the atmosphere also cause lime deposits on the ­concrete surface to dissolve. LANXESS Deutschland GmbH has published a brochure about efflorescence on concrete, which is available to customers on request. Weathering of the cured cement matrix There is a sludge layer consisting of aggregate fines and ­cement on the surface of the concrete. Its thickness ­depends on the formulation, method of compaction, etc. This l­ayer (cured cement matrix) is gradually weathered away and, after a few years, the aggregate particles on the surface b ­ ecome more exposed and thus contribute more to the overall color of the product. The photo below shows that the color ­changes in pigmented building materials are relatively small. These changes are due to the color of the aggregate and the ­different way light is reflected. Fig. 17: New and weathered paver, on which the color of the sand is evident Lightness Concrete paving Weathering time LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 15 Fig. 18: Concrete walling blocks after 25 years of outdoor weathering Weather stability of pigments Provided that weather-stable pigments such as Bayferrox® and chromium oxide green (i. e. oxidic) pigments are used for coloring building materials, their color can be expected to last. This is based on experience from over a quarter of a ­century of systematic trials of the stability of pigmented building materials. In these studies, which looked at a variety of issues, it was also found that only outdoor natural weathering tests can truly provide reliable information on the weather ­stability of pigments used in building materials. The photo above shows that the color changes in ­pigmented building materials are relatively small. Compared with the unweathered specimen in the foreground, concrete bricks weathered for 25 years show very little change apart from slight soiling of the surface. The long-term weather stability can be completely different, though, depending on the pigment selected. In a maritime climate, for example, the color of concrete ­paving stones pigmented with carbon black faded after a ­relatively short weathering period and only stones pigmented 16 with iron oxide black exhibited the required color stability. This proved that a number of pigments (e. g. carbon blacks and various organic pigments) do not provide adequate weather stability (Fig. 19). Fig. 19: Weather stability of black pigments 3% Large particle carbon black 3% Fine particle carbon black unweathered LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 3% Bayferrox® 360 weathered 3% Bayferrox® 330 unweathered THE TECHNICAL PROPERTIES OF COLORED CONCRETE Standards The requirements relating to pigments for coloring building materials are specified in various standards. The ­relevant standard in Europe is EN 12 878 “Pigments for the colouring of building materials based on cement and/or lime”, while ASTM C 979 “Pigments for integrally colored concrete” applies in the United States. EN 12 878 Conformity is confirmed by means of factory production ­controls and the resulting certification by a notified body (CE mark). The notified body issues certificates that replace the certificates of conformity used previously. The CE mark, which is also placed on the packaging, documents the product’s conformity. EN 12 878 specifies additional testing requirements for reinforced concrete (Cat. B), in particular relating to test ­ frequency, a lower tolerance for chloride content and a ­ low proportion of water-soluble components. To satisfy the ­requirements of the standard, including as regarding documentation, LANXESS lists these products separately as ­special formulations. The test certificate lists the required ­data for each batch and includes a declaration of the intended use. ASTM C 979 This standard establishes the requirements for pigments used in colored concrete all of which are fulfilled by B ­ ayferrox® & ® Colortherm . Conclusion: LANXESS pigments satisfy the requirements of EN 2878 and ASTM C 979. Concrete strength and curing behavior of cement Besides dealing with questions regarding the testing of pigments, EN 12 878 also specifies thresholds for the extent to which pigments may influence the curing behavior of cement and the strength of concrete. Konformitätserklärung Declaration of conformity Déclaration de conformité Declaracion de conformidad Declaração de conformidade DIN EN 12 878 : 2014 LANXESS Deutschland GmbH Inorganic Pigments PBD - GCC Construction Geb. R 54 / Raum 024 47812 Krefeld, Deutschland Telefon: Telefax: +49 2151 88-7741 +49 2151 88-4133 Email: [email protected] Internet: www.lanxess.com www.bayferrox.de LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 17 Concrete consistency Pigments are made up of very fine particles. The shadecard shows precise details about the mean particle size, which can vary considerably depending on the grade. As a rough guide, pigments are approximately 10 – 20 times finer than cement. Consequently, pigment processors must ask themselves whether adding such a fine product has some influence on the water required by the concrete. The amounts of Bayferrox® Black and Bayferrox® Red pigments­added in practice have virtually no effect in this respect. Iron oxide yellow pigments differ from the above-mentioned black and red iron oxides in that they have a needle-shaped structure and can therefore adsorb more ­ water on their surface. However, this effect only becomes n ­ ­oticeable at pigment concentrations above approx. 4 – 5 %. This value is ­generally not exceeded when using pigments with a high ­tinting strength, such as Bayferrox® Yellow grades. The higher water adsorption of the yellow pigments is therefore of only limited interest to concrete manufacturers. If larger amounts of iron oxide yellow pigments are added to the concrete, however, the water bound to the pigment surface results in a tangible reduction in the effective water-cement ratio and associated changes in the consistency of the concrete. To achieve the same slump as uncolored concrete, the amount of water added must be increased, which may adversely affect the strength of the concrete. Fig. 20: Slump test comparing unpigmented and pigmented in-situ concrete Slump (water-cement ratio 0.56) 18 unpigmented 3 % Bayferrox® 920 3 % Bayferrox® 110 3 % Bayferrox® 319 d = 39 cm d = 36 cm d = 38 cm d = 39 cm 6 % Bayferrox® 920 6 % Bayferrox® 110 6 % Bayferrox® 319 d = 32 cm d = 36 cm d = 37 cm LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete QUALITY AND ADDED VALUE On closer examination, it quickly becomes clear that concrete and pigment technology are fundamentally different technical disciplines. If concrete manufacturers have a lab, this is normally restricted to performing technical concrete tests and developing concrete formulations. Such labs are not, however, set up to deal with issues relating to coloring, such as the task of producing concrete in a highly specific color. Nor, generally speaking, are they equipped to deal with rationalization issues regarding the number of pigments required for the concrete manufacturer’s color range, or with issues relating to the color consistency of building materials. This is where the pigment manufacturer’s specialists come in. The Global Competence Center Construction of ­L ANXESS Inorganic Pigments offers customers a comprehensive g ­ lobal application engineering service that not only covers color matching under realistic conditions, but also all issues relating to the use of pigments as well as mixing and metering technology. This enables LANXESS to help customers significantly improve the quality of their end product. Middelburg Town Hall, Netherland; pigmented with Bayferrox® 330 LANXESS INORGANIC PIGMENTS – processing instructions for coloring concrete 19 Health and safety information Appropriate documentation was compiled with information on the health and safety measures that have to be observed in handling the LANXESS products mentioned in this brochure. For materials mentioned here that are not LANXESS products, the operational hygiene and other safety measures recommended by the respective manufacturers must be observed. Before working with these products, you must read and familiarise yourself with the available information on their dangers, proper use and handling. This point is of decisive importance. Information is available in various forms: such as safety data sheets, product information and product labels. Please contact your LANXESS representative in Germany or the Department of Regulatory Affairs and Product Safety of LANXESS Deutschland. For business in the USA, please contact the LANXESS Product Safety and Regulatory Affairs Department in Pittsburgh, Pennsylvania.­­ LANXESS Deutschland GmbH Business Unit Inorganic Pigments Rheinuferstraße 7-9 47829 Krefeld Germany Tel. +49 2151 88-7504 Fax +49 2151 88-4133 www.lanxess.com www.bayferrox.com Information on Regulatory Compliance For some end use purposes of the products found in this brochure, the applicable regulations must be observed, including those of the FDA, BfR, NSF, USDA and CPSC. If you have any questions regarding the approval status of these products, please contact your representative at LANXESS Deutschland GmbH or the Department of Regulatory ­Affairs and Product Safety of LANXESS Deutschland GmbH or, for business in the USA, your representative at LANXESS ­Corporation, the LANXESS Regulatory Affairs Manager in Pittsburgh, Pennsylvania. How and for which purposes you utilise our products, our technical support and our i­nformation (oral, written or through product assessments) is beyond our control. The same applies for suggested formulations and recommendations. Therefore it is indispensable that you check our products, our technical support and our information for their suitability for the intended processes and purposes. The application-specific analysis must encompass at least suitability tests in regard to technical as well as health, safety and environmental aspects. Such testing has not necessarily been done by us. Unless agreed to otherwise in writing, all products are sold exclusively in accordance with our general terms and conditions for sale and delivery. Information and technical support are provided without warranty (we reserve the right to make changes at any time). It is expressly agreed that you release us from any possible liability resulting from the use of our products, technical support and information due to fault, contract or other reasons and that you assume this liability yourself. Any statements and recommendations not contained in this brochure are not authorised and are not binding for us. None of the information in this brochure is to be interpreted as a recommendation to use the products in any way that violates commercial proprietary rights such as patents in regard to any ­materials or their use. Furthermore, neither ­explicitly nor implicitly is any licence granted under commercial proprietary rights such as ­patents. Edition 04/2016 Bayferrox® is a registered trademark of Bayer AG, Leverkusen, Germany. Colortherm® is a registered trademark of the LANXESS Group.